# Ultra-Thin Carbon Films: The Rise of sp 3 -C-Based 2D Materials?

Fabrice Piazza, Marc Monthioux

► To cite this version:

Fabrice Piazza, Marc Monthioux. Ultra-Thin Carbon Films: The Rise of sp 3 -C-Based 2D Materials?. C - Journal of Carbon Research, 2021, 7, pp.30. 10.3390/7020030 . hal-03431060

HAL Id: hal-03431060

https://hal.science/hal-03431060

Submitted on 16 Nov 2021

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
<figure><img src="image_2.png" /></figure>

Editorial

# Ultra-Thin Carbon Films: The Rise of sp³-C-Based 2D Materials?

Fabrice Piazza <fnref n="1" />,* ID and Marc Monthoux <fnref n="2" /> ID

We warmly thank all the colleagues who have enthusiastically participated in the project of this Special Issue on "2D Ultra-Thin Carbon Films", considering a globally unfavorable context characterized by (i) a myriad of publication options; (ii) strong pressure, by the highly competitive research (and researcher) funding and evaluation system, to publish in high impact factor journals, specifically for topics of worldwide interest; and (iii) all sorts of restrictions imposed by the sanitary crisis. Likewise, we are very grateful to all reviewers for their time and altruism considering this very particular context.

This issue focuses on different aspects of 2D Ultrathin Carbon Films. Both sp<fnref n="2" />-bonded carbon and sp³-bonded carbon materials are considered, although the latter are emphasized. We believe that this characteristic may be of particular interest considering the countless issues and reviews already dedicated exclusively to graphene. Moreover, although graphene initiated the booming field of two-dimensional (2D) and layered materials, since the seminal paper by Geim and Novoselov in 2004, which earned them the 2010 Nobel Prize in Physics, the craze for graphene might start to fade (see Figure 1).

<figure><img src="image_3.png" /></figure>

check for
updates

**Citation:** Piazza, F.; Monthoux, M. Ultra-Thin Carbon Films: The Rise of sp³-C-Based 2D Materials? C **2021**, *7*, 30. https://doi.org/10.3390/c7020030

Received: 12 March 2021

Accepted: 22 March 2021

Published: 25 March 2021

**Publisher's Note:** MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations.

<figure><img src="image_4.png" /><figcaption>**Figure 1.** Number of published scientific articles per year since 2012 referring to graphene (black squares), TMDs (red circles) or MXenes (green triangles) in their abstract (source: Scopus, February 2021).</figcaption></figure>

<figure><img src="image_5.png" /></figure>

**Copyright:** © 2021 by the authors. License MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

Indeed, no matter how beautiful the material is, single graphene is vitiated by a major deficiency, i.e., the lack of an electronic band gap. Due to this, other mono-elemental materials such as phosphorene [1] or silicene [2], and compounds such as transition metal dichalcogenides (TMDs) [3] or transition metal carbides, nitrides, or carbonitrides (MXenes) [4], have emerged and now increasingly attract the attention of the scientific community (Figure 1), dragging many research teams worldwide out of the carbon field. However,

<footnote n="1">¹ Laboratorio de Nanociencia, Pontificia Universidad Católica Madre y Maestra, Apartado Postal 822, Santiago de los Caballeros, Dominican Republic</footnote>

<footnote n="2">² Centre d'Elaboration des Matériaux et d'Etudes Structurales (CEMES), CNRS, Université de Toulouse, BP 94347, 31055 Toulouse, France; marc.monthoux@cemes.fr</footnote>

<footnote>* Correspondence: fpiazza@pucmm.edu.do</footnote>
this is forgetting that carbon has kept providing scientific breakthroughs over the past
35 years.

The high interest in 2D materials is illustrated by the corresponding significant increase
in the number of published scientific articles and the multiplication of dedicated conference
sessions every year. Between 2015 and 2020, the number of published scientific articles
per year which were indexed in Scopus and which were referring to 2D materials in their
abstract has more than doubled, increasing from ~3400 to ~7300. The Materials Research
Society will organize a symposium focusing on 2D materials during the 2021 Virtual
MRS Spring Meeting and Exhibit (Symposium NM07-Beyond Graphene 2D Materials—
Synthesis, Properties and Device Applications) following the success of similar symposia at
the 2019 and 2020 MRS Fall meetings. 2D materials also get a dedicated journal since 2014
(see [5]), and a European experimental pilot line devoted to 2D materials was just launched
in January 2021 as an initiative of the Graphene Flagship. Despite the interest in graphene
is still quite high and remains well ahead of others (Figure 1) thanks, in particular, to the
incorporation of nitrogen in the graphene lattice for energy storage applications and more
recently twisted bi-layer graphene (TBG) for its superconductivity (1223 and 181 articles in
2020, respectively), the number of articles dedicated to graphene has started to decrease
(by 1.4% from 2019 to 2020), while the current craze generated by newcomer materials
is obvious.

A major motivation for 2D-material research is the synthesis of high-quality materials for electronic and optoelectronic applications. However, as stated in a recent article discussing a roadmap for electronic grade 2D materials [5], "for industrial production, 2D layer synthesis and engineering must lead to 'exfoliation-quality' 2D layers at the wafer scale". Hence, as pointed out by Luigi Colombo (Texas Instruments) some years ago during his invited talk at the MRS Fall meeting, it will be far more challenging to produce (and to integrate into devices) at wafer-scale an electronic grade 2D-compound material than a mono-elemental one. This is still a robust hypothesis for which we understand that 2D ultrathin carbon materials (2DC) offer a lot of promises for this sector of applications, especially as the field has recently evolved with new promising 2DC (besides TBG), namely 2D sp³-bonded carbon materials. Another imperative incentive is the necessity of using materials and production processes, which are safe and compatible with sustainable development. As a matter of fact, carbon is one of the most abundant elements on Earth, whereas some elements necessary for other 2D materials, such as copper (or tin or indium) have started to become scarce. Additionally, our modern lifestyle produces excess gaseous forms of carbon (CO₂, CH₄), which are detrimental to the planet because of their significant contribution to the green-house effect. Hence, capturing the gaseous carbon forms into carbon materials is a promising double-winning strategy to consider. Likewise, 2DC can be produced by using green mass-production routes, which are also CMOS-compatible. 2DC materials open the door to significant advances in driving technologies, where they can compete with more complex materials, which are more challenging to manufacture and integrate, such as BN, TMDs, or MXenes. Further developments consisting of combining 2DC materials with each other, such as combining graphene with diamanoid, could motivate intense research to develop carbon-based electronics where both carbon materials would play a major role.

In 2018, in their perspective on current achievements and future challenges for carbon
science, the editors of the journal *Carbon* considered that one experimental challenge that
remained was the development of a bulk synthesis method for 2D diamonds and that
a real breakthrough would be to use chemical vapor deposition (CVD) processes such
as hot filament CVD in the presence of H₂ and CH₄, to yield scalable synthesis of 2D
or 1D diamonds [6]. Actually, it was recently shown that hot filament CVD-promoted
hydrogenation processes can be successfully used to induce the partial or full sp² to sp³
conversion of carbon atom hybridization in 2D graphenic systems at low pressure and at
low temperature to synthesize 2D crystalline sp³-bonded carbon materials [7–11]. These
results open the door to mass production of a variety of stable 2DC materials such as
diamanes, diamanoids, and diamanoid/graphene hybrids (including TBG configurations),
merely by changing the type of graphenic 2DC to start with (from coherently stacked 2LG to few-layer graphene). Meanwhile, a major advantage is the use of the hot-filament-assisted CVD process, which is already a well-established method for the industrial production of other crystalline *sp*³-bonded carbon materials, such as diamond films.

This is why the focus of this Special Issue is on new arising carbon materials, namely TBG and *sp*³-carbon-related materials, the latter being wide band-gap semiconducting materials, which include genuine diamane, F-diamane, N-diamane, diamanoids, and amorphous carbon layers with high *sp*³-bonded carbon fraction. Genuine diamane consists of two crystalline *sp*³-bonded carbon layers, for which half of the carbon atoms are hydrogenated while the other half bond the two layers to each other. Diamanoids are crystalline *sp*³-bonded carbon materials such as diamane, but they are composed of more than two layers while only the two outer ones are hydrogenated. The issue includes a contribution on F-graphene for the possibility of converting the material into F-diamane. The issue comprises a research article and four review articles. Experimental and first-principle works are included. Altogether, the manuscripts collected cover a variety of topics including synthesis, characterization, physical properties, applications, and cyto-compatibility.

We introduce the contributions to this Special Issue starting with *sp*²-bonded carbon materials and continuing with *sp*³-bonded carbon materials in order to follow the chronology of historical developments. Regarding the *sp*²-bonded 2DC materials, the issue includes a review on Raman spectroscopy of TBGs [12]. Moutinho and coworkers review the main important effects observed in the Raman spectra of TBGs and twisted graphene/other phase heterostructures, with different twisting angles and recorded with different laser excitation energies. New Raman peaks appear in the Raman spectra of TBGs and twisted graphene heterostructures. Their positions depend on the twisting angle θ so that they can be used to provide a rough estimate of the latter. A large enhancement of the Raman G band occurs when the energy of the excitation laser line matches the energy separation between the van Hove singularities in the density of states (DOS) of TBGs with θ from 9° to 17°, when they are probed using laser excitation energies in the visible range. In the case of TBGs with low or high twisting angles, the Raman G band intensity is smaller than twice that of single-layer graphene. These results show that the G band enhancement is associated with the smaller quasi-periodic Moiré unit cell and not with the commensurate superlattice unit cell. It has been reported recently that the enhancement of the extra peaks associated with the Moiré patterns has two different resonance processes. Some peaks are enhanced, both below or above the G band position, for excitation laser energies where the G band is not enhanced. This resonance mechanism is called the intralayer electron-phonon process and is similar to the double resonance Raman process that activates the disorder-induced D band, but, in the case of TBGs, the momentum conservation of the double-resonance process is provided by the periodic potential of the Moiré superlattice.

Ahmad and coworkers provide a review on the preparation and applications of fluorinated graphenes [13]. Two preparation routes are considered: (i) the addition of fluorine atoms and (ii) the exfoliation of graphite fluoride. The chemical bonding in fluorinated graphene, the related properties, and a selection of applications are discussed. These include lubrication, energy storage, and gas sorption and sensing. The authors also address cytotoxicity issues, a very important field that is still often neglected when introducing new materials. However, a good reason for the latter is that it requires a totally different field of competence. Hence, the interest of a team with the needed expertise has to be attracted, which is hard to achieve as long as the actual technological interest of the targeted new material is not fully demonstrated. In the case of cells put in contact with fully fluorinated graphene, the cell viability is shown to decrease. In a general way, the biological response depends on the fluorine content. The adhesion and aggregation of blood platelets are shown to decrease with an increase in the fluorine content. On the other hand, a favorable antibacterial activity against *Escherichia coli* of partially fluorinated graphene is also evidenced.
The other articles concern sp³-carbon-related materials, starting with the research paper by Pakornchote and coworkers, which deals with the modification of electronic and elastic properties of 2D [110] diamond by nitrogen substitution [14]. The authors theoretically demonstrate that 2D diamond derived from the [110] direction exhibiting a washboard conformation can also be stabilized by N-substitution, as was previously shown in the case of 2D diamond that is derived from the [111] direction. Three structural models of washboard-like carbon nitrides of different compositions (C₆N₂, C₅N₃, and C₄N₄) are studied together with the fully hydrogenated washboard-like diamane (C₈H₄). The results show that the band gap of washboard-like carbon nitrides is open if no dangling bond is left to be passivated. When comparing with the hydrogenated phase, the N-substituted phases have higher elastic constants and bulk modulus, suggesting that they are possibly harder than diamane, which is fully hydrogenated.

It can be seen that the previous paper includes a comparison with a diamane material. This reveals that diamanes and diamanoids are becoming important materials to the field of 2DC. Indeed, the application potential of diamanes and diamanoids is broad. Besides band-gap engineering, they could be used as an active laser medium in nano-optics. Due to its expected high thermal conductivity, they may be used in thermal management devices. Calculations have shown that diamane is a better host system for single-photon emission than diamond. Diamane-related materials are also expected to be mechanically very strong; therefore, they may be very attractive for ultrathin protective coatings, ultrahigh-strength components in composite materials for aerospace applications for instance, and nano-electromechanical systems. Due to the expected low friction coefficient of the hydrogenated surface, diamanoids may also be used to improve the wear resistance of coated mechanical parts and anti-adhesion surface properties. The expected strength, low coefficient of friction, and bio-compatibility could render diamane-related materials very competitive as building materials to make lower power and miniaturized electronics and biomedical devices. A diamane nanoribbon resonator was calculated to be better than single-layer graphene, bi-layer graphene, MoS₂, or other 2D-nanomaterial resonators (at least for the temperature range from 1 K to 300 K) [15]. Heterostructures of graphene and diamanoid would be attractive for tunnel devices, optical linear waveguides, high-efficiency optoelectronic sensors, lithium batteries, and supercapacitors.

Therefore, the next two papers deal with diamane and diamanoids. It includes a contribution from the group that pioneered the research on these new materials by being the first to hypothesize them [16,17]. Chernozatonskii and coworkers provide a review on theoretical and experimental studies on diamane-related materials with various atomic structures and types of functionalization (with either hydrogen or fluor) [18]. This article includes recent results on diamane systems exhibiting Moirés, i.e., involving domains with slight rotational misorientations. It is shown that diamanes are mechanically stronger than graphene and graphane and have wide bandgaps ranging from 3.1 to 4.5 eV depending on the structure. The potential applications are briefly reviewed.

Finally, this Special Issue ends with a review on the experimental synthesis of genuine diamanes and diamanoids including diamanoid/TBG [11]. Genuine diamane is prepared from the exposure of bi-layer graphene (2LG) to hydrogen radicals produced by the hot-filament process at low pressure and temperature. A sharp sp³-bonded carbon stretching mode, assigned to the diamond/lonsdaleite stretching mode between sp³-C (diamond E₂g mode; lonsdaleite A₁g and E₂g modes) is observed in ultraviolet Raman spectra, while no sp²-bonded carbon peak is simultaneously detected. By replacing 2LG with few-layer graphene (FLG), diamanoid/graphene hybrids are formed from the partial conversion of FLG due to the prevalent Bernal stacking sequence. Raman spectroscopy, electron diffraction, and Density Functional Theory calculations show that partial conversion generates TBG located at the interface between the upper diamanoid domain and the non-converted graphenic domain underneath. Carbon-hydrogen bonding in the basal plane of hydrogenated FLG, where carbon is bonded to a single hydrogen over an area of 150 µm², is directly evidenced by Fourier transform infrared microscopy, and the actual full
hydrogenation of diamane is supported by first-principle calculations. Raman mapping and FTIR observations indicate the hydrogenation and subsequent $sp^3$ conversion over surface areas of up to 2000 $\mu m^2$. Importantly, it is believed that dimensions are only limited by the dimensions of the starting material, not by the process. Therefore, those results open the door to mass production of diamanes, diamanoids, and diamanoid/graphene hybrids by means of the hot-filament-assisted CVD process. It is believed that the key to producing homogenous diamane films is to start with very high-quality 2LG material, ideally, single-crystal AB flakes as large as possible. Finally, from a more fundamental standpoint, those recent results should reanimate a 50-years-long discussion on the origin of some crystalline $sp^3$-bonded carbon grains in extraterrestrial environments.

2D materials will definitely play an important role in the close future of technology. What part will carbon materials (2DC) take in it? We do believe that this Special Issue is merely one hint among many others that show that 2DC will maintain a top level of research interest. There are two major reasons for this: (1) as opposed to carbon, alternate non-carbon materials may exhibit fatal drawbacks in the mid/long term with respect to sustainability (scarcity of feedstock sources, intrinsic toxicity) and processing difficulty; (2) the versatility of carbon makes it highly inventive. Beyond graphene, this Special Issue shows several examples of the potential ability of $sp^3$-carbon-related materials to fulfill electronics needs. There might be the future of carbon for such applications, which was unexpected a few years ago, when only graphene was considered. This would not be the first time there was such a change of mind. Recall that not so long ago, energy storage could not do without the most conductive carbon material, namely graphite, while other carbon materials were discarded because of their low electrical conductivity; however, nowadays, in spite of this, using so-called "hard" carbons (i.e., graphenic carbon materials unable to graphitize) instead of graphite is currently the route that is boosting the research activity in this field. Hence, with fullerenes, nanotubes, and graphenes, $sp^2$ carbons might have given their best, while, for decades, $sp^3$ carbons were not seen able to give better than nanodiamonds. The time may have come for $sp^3$-carbon-based 2D materials.

We were very pleased to guest-edit this Special Issue, and we hope that it will reach the widest audience of materials science researchers, in particular those working in the field of carbon-related materials, and that it will contribute to boosting further scientific and technological advances.

**Author Contributions:** Both authors contributed equally to this manuscript. Both authors have read and agreed to the published version of the manuscript.

**Funding:** F.P. acknowledges funding from the Ministry of Higher Education, Science and Technology of the Dominican Republic, MESCyT (2018-2019 FONDOCyT program). Partial funding by the EUR grant NanoX #ANR-17-EURE-0009 in the framework of the "Programme des Investissements d'Avenir" is also acknowledged.

**Conflicts of Interest:** The authors declare no conflict of interest.

## References

1. Castellanos-Gomez, A. Black Phosphorus: Narrow Gap, Wide Applications. *J. Phys. Chem. Lett.* **2015**, *6*, 4280-4291. [CrossRef] [PubMed]

2. Oughaddou, H.; Enriquez, H.; Tchalala, M.R.; Yildirim, H.; Mayne, A.J.; Bendounane, A.; Dujardin, G.; Ali, M.A.; Kara, A. Silicene, a Promising New 2D Material. *Prog. Surf. Sci.* **2015**, *90*, 46-83. [CrossRef]

3. Manzeli, S.; Ovchinnikov, D.; Pasquier, D.; Yazyev, O.V.; Kis, A. 2D Transition Metal Dichalcogenides. *Nat. Rev. Mater.* **2017**, *2*, 1-15. [CrossRef]

4. Venkateshalu, S.; Grace, A.N. MXenes—A New Class of 2D Layered Materials: Synthesis, Properties, Applications as Supercapacitor Electrode and Beyond. *Appl. Mater. Today* **2020**, *18*, 100509. [CrossRef]

5. Briggs, N.; Subramanian, S.; Lin, Z.; Li, X.; Zhang, X.; Zhang, K.; Xiao, K.; Geohegan, D.; Wallace, R.; Chen, L.-Q.; et al. A Roadmap for Electronic Grade 2D Materials. *2D Materials* **2019**, *6*, 022001. [CrossRef]

6. Bianco, A.; Chen, Y.; Chen, Y.; Debjit, G.; Hurt, R.H.; Kim, Y.A.; Koratkarhi, N.; Meunier, V.; Terrones, M. A Carbon Science Perspective in 2018: Current Achievements and Future Challenges. *Carbon* **2018**, *132*, 785-801. [CrossRef]

7. Piazza, F. $Sp^3$-Bonded Carbon Materials, Methods of Manufacturing and Uses Thereof. WO Patent 2019/233901, 5 June 2018.
8. Piazza, F.; Gough, K.; Monthioux, M.; Puech, P.; Gerber, I.; Wiens, R.; Paredes, G.; Ozoria, C. Low Temperature, Pressureless sp² to sp³ Transformation of Ultrathin, Crystalline Carbon Films. *Carbon* **2019**, *145*, 10–22. [CrossRef]

9. Piazza, F.; Monthioux, M.; Puech, P.; Gerber, I. Towards a Better Understanding of the Structure of Diamanoïds and Dia-manoïd/Graphene Hybrids. *Carbon* **2020**, *156*, 234–241. [CrossRef]

10. Piazza, F.; Puech, P.; Gerber, I.; Cruz, K.; Monthioux, M. Raman Evidence for the Successful Synthesis of Diamane. *Carbon* **2020**, *169*, 129–133. [CrossRef]

11. Piazza, F.; Monthioux, M.; Puech, P.; Gerber, I.C.; Gough, K. Progress on Diamane and Diamanoid Thin Film Pressureless Synthesis. *C* **2021**, *7*, 9. [CrossRef]

12. Moutinho, M.V.O.; Venezuela, P.; Pimenta, M.A. Raman Spectroscopy of Twisted Bilayer Graphene. *C* **2021**, *7*, 10. [CrossRef]

13. Ahmad, Y.; Batisse, N.; Chen, X.; Dubois, M. Preparation and Applications of Fluorinated Graphenes. *C* **2021**, *7*, 20. [CrossRef]

14. Pakornchote, T.; Ektarawong, A.; Pinsook, U.; Bovornratanaraks, T. Modifying Electronic and Elastic Properties of 2-Dimensional Diamond by Nitrogen Substitution. *C* **2021**, *7*, 8. [CrossRef]

15. Zheng, Z.; Zhan, H.; Nie, Y.; Xu, X.; Qi, D.; Gu, Y. Single layer diamond-A new ultrathin 2D carbon nanostructure for mechanical resonator. *Carbon* **2020**, *161*, 809–815. [CrossRef]

16. Chernozatonskii, L.A.; Sorokin, P.B.; Kvashnin, A.; Kvashnin, D.G. Diamane: Simulation of the structure and properties. *J. Exp. Theor. Phys. Lett.* **2009**, *90*, 134–138. [CrossRef]

17. Chernozatonskii, L.A.; Sorokin, P.B.; Kuzubov, A.A.; Sorokin, B.P.; Kvashnin, A.G.; Kvashnin, D.G.; Avramov, P.V.; Yakobson, B.I. Influence of size effect on the electronic and elastic properties of diamond films with nanometer thickness. *J. Phys. Chem. C* **2011**, *115*, 132–136. [CrossRef]

18. Chernozatonskii, L.A.; Demin, V.A.; Kvashnin, D.G. Fully Hydrogenated and Fluorinated Bigraphenes-Diamanes: Theoretical and Experimental Studies. *C* **2021**, *7*, 17. [CrossRef]